J Mol Model (2011) 17:607–619DOI 10.1007/s00894-010-0755-z ORIGINAL PAPERModeling and analysis of the compatibilityof polystyrene/poly(methyl methacrylate) blendswith four inducing effectsDan Mu & Jian-Quan Li & Yi-Han ZhouReceived: 8 February 2010 / Accepted: 1 April 2010 / Published online: 5 June 2010# Springer-Verlag 2010Abstract The compatibility of polystyrene (PS) and poly Introduction(methyl methacrylate) (PMMA) blends was studied over awide range of compositions at 383, 413 and 443 K, Polymer blend systems play an important role in the plasticrespectively, by atomistic and mesoscopic modeling. All industry because they can be tuned to have a betterthe calculated Flory–Huggins interaction parameters combination of physical properties than the correspondingshowed positive values; furthermore, they were all above homopolymers. The process of physical blending is muchthe critical Flory–Huggins interaction parameter value, easier to perform than chemical blending (e.g., grafting),which means that the PS/PMMA blends were immiscible. and the former is also more economical. As a general rule,Both the addition of a block copolymer and the introduction the aim of blending is to obtain a product with new or betterof a shear field influenced the phase morphologies of the properties. Because of the different physical properties ofblends, while the degree of influence depended on the candidate polymers, it is not always easy to obtaincompositions of the blends. The study of PS/PMMA blends completely miscible polymer mixtures. When the compo-doped with nanoparticles showed that the mesoscopic phase nents of polymers can form energetically favorable inter-was influenced by not only the properties of the nano- actions, such as hydrogen bonding, dipole interactions, etc.,particles, such as their size, number and number density, it is possible to obtain a miscible blend. For immisciblebut also the compositions of the blends. The effect of the blends, adding interferents is a common method ofsurface roughness of the planes on the phase separation of changing the microscopic morphology. This improves thethe blends was also studied. blend miscibility and thus enhances its properties. Polystyrene (PS) and poly(methyl methacrylate)Keywords PS/PMMA blend . Inducing effect . Phase (PMMA) are conventional model systems in polymermorphology . Nanoparticle science. PS/PMMA blends are a well-known immiscible combination [1-8], and their bulk and surface phase separation has been observed [9, 10]. Immiscible blendsD. Mu (*) are known to have properties combining those of theirDepartment of Chemistry, Zaozhuang University, component polymers, and also to have segregated structuresShandong 277160, Chinae-mail: email@example.com with domains that are predominantly formed from the individual homopolymers. It has been shown that changingJ.-Q. Li the relative homopolymer proportions in such blends canPhysics and Electronic Engineering Department, change the domain structure, surface morphology, and evenZaozhuang University,Shandong 277160, China the phase morphology [11-13]. Some contradictory results can be found in the literatureY.-H. Zhou regarding the miscibilities of certain polymers and theNational Analytical Research Center of Electrochemistry possibility of predicting miscibility from surface tension orand Spectroscopy, Changchun Institute of Applied Chemistry,Chinese Academy of Sciences, from parameters derived from it. These contradictions canChangchun, China be attributed to several reasons. Firstly, the structures and
608 J Mol Model (2011) 17:607–619the properties of partially miscible polymer blends depend blending materials and planes or doped nanoparticles.on the processing conditions used, which may influence Furthermore, in the study of the compatibility of PEO/PMMAconclusions about polymer compatibility when they are blends in our former work, the MesoDyn simulation methoddeduced from macroscopic properties or from the structure was successfully applied to detect the phase morphologies ofof the blend. Secondly, methods that can be used to predict PEO/PMMA blends. From a theoretical point of view, thesemiscibility are limited [14, 15]. For example, various results clarified several conflicting conclusions of differentexperimental difficulties can be encountered during the experiments . Therefore, the MesoDyn method has beendetermination of the Flory–Huggins interaction parameter, shown to be reliable when dealing with PS/PMMA blends.χ, which can be used to characterize the strength of the The mesoscale simulation process used in this paper wasinteraction between the polymers. χ can be determined by carried out with the MesoDyn module in the Material Studiovarious methods, such as inverse gas chromatography, commercial software provided by Accelrys.solvent diffusion, or the dependence of composition onmechanical properties, but all of these methods have theirdrawbacks. Finally, when blend systems have two calori- Simulation details, results and discussionsmetric Tg values, it does not necessarily indicate that theircomponents are immiscible . Fortunately, computer This paper consists of two parts: calculations performed viacalculations and simulations have become available as (1) molecular dynamic (MD) simulations and (2) mesoscopicefficient methods of solving these experimental problems. simulations. The intermediate parameter connecting the This paper is divided into two main parts. The first part microscale and the mesoscale is the Flory–Huggins param-is about the calculation of typical thermodynamic param- eter, χ. MD simulation is used to accurately study bulketers, such as the solubility parameter, of the studied polymer properties when this is difficult to do experimental-systems via a microscopic calculation method, and com- ly. Although MD simulation is widely used nowadays, it isparing those calculated parameters with experimental data difficult to detect the phase separation of blends via ain order to maintain a high level of accuracy in further microscopic method, such as MD simulation. Therefore, it iscalculations and simulations; the second part describes necessary to combine it with a mesoscopic method, such asmesoscopic dynamics simulations of several kinds of MesoDyn simulation, to perform a full study of polymerinducing effects that can change the phase morphologies blends from the microscale to the mesoscale.of PS/PMMA blends. Mesoscale structures are of theutmost importance during the production processes of Atomistic molecular simulationmany materials, such as polymer blends, block copolymersystems, surfactant aggregates in detergent materials, latex Model and simulationparticles, and drug delivery systems. Mesoscopic dynamics models have been receiving increas- The selection of the representative chain length (Nmon) wasing attention recently, as they form a bridge between our primary task. This simulation process was carried out atmicroscale and macroscale properties [17-20]. Mesoscopic room temperature (298 K) on an SGI workstation bydynamics (MesoDyn) [21-23] and dissipative particle dy- following the MD procedure in the commercial Cerius2namics (DPD) [24, 25] methods both treat the polymer chain package program provided by Accelrys.at a mesoscopic level by grouping atoms together and then The simulation processes (including the construction of thecoarse-graining them to be persistent-length polymer chains. models) were the same for both PS and PMMA, so we will useThese two mesoscopic modeling methods increase the scale an atomistic chain length N of 10 for PS as an example hereof the simulation by several orders of magnitude compared to describe the simulation process in detail. Initially, thewith atomistic simulation methods. MesoDyn utilizes dy- proposed polymer chain structure was generated using thenamic mean-field density functional theory (DFT), in which rotational isomeric state (RIS) model of Flory , whichthe dynamics of phase separation can be described by describes the conformations of the unperturbed chains. ThreeLangevin-type equations to investigate polymer diffusion. PS polymer chains were then generated following the sameThermodynamic forces are found via mean-field DFT, using principle, each with ten repeating units; they were then putthe Gaussian chain as a model. The most important into a simulation box with a density of 1.05, which is themolecular parameter is the “incompatibility parameter” χN, density of bulk PS . Minimization was then done usingwhere χ is the Flory–Huggins interaction parameter and N is the conjugate gradient method (CGM) with a convergencethe degree of polymerization. level of 0.1 kcal mol−1 Å−1 until the energy reached a However, owing to the soft interaction potential of the minimum. This minimized configuration was refined by MDDPD method, it is not suitable to apply the DPD method in our simulation for 30 ns under constant temperature and densitywork, especially when dealing with the interactions between (NVT ensemble). A time step of 1 fs was used to ensure the
J Mol Model (2011) 17:607–619 609stability of simulation. The Nosé–Hoover  thermostat ina canonical ensemble was used to create the canonicalmolecular dynamics trajectories, and the COMPASS forcefield was chosen to deal with such a condensed state system[31-33]. The spline treatment of van der Waals (VDW)interactions was chosen, with a spline window of between 11and 12 Å. The Ewald summation , an accurate method ofcalculating long-range interactions, was applied in order tocalculate long-range electrostatic interactions. Next, therefined polymer was annealed in the temperature range from383 K (above 373 K , the Tg of PS) to 443 K (below513 K , the melting temperature Tm of PS) in steps of10 K for 50 cycles. The simulation time for each annealingcycle was set to 2 ns, and the system was minimized at thebeginning of each annealing cycle. Because such oligomersalways have strong end–end interactions, a system consisting Fig. 1 The solubility parameter for different PS chain lengthsof oligomers is different from a real polymeric system. Thus,an MD simulation was executed with the NPT (with constanttemperature and pressure) ensemble for 20 ns; furthermore, numbers of repeating units of PMMA. These becomeMD simulations with a repeating ensemble cycle from NVT constant from N=60 onwards, and they are 6.40% smallerto NPT were carried out three times with a simulation time of than the experimental results. This may result from the20 ns for each cycle to reduce the end–end interactions presence of a bulky CH3 group in PMMA, which alsosufficiently. Finally, an MD simulation was executed with restricts free rotation around the C–C bond of its backbone.the NVT ensemble for 30 ns at 298 K to collect data. In The fact that the calculated relaxation times weregeneral, about 200 ns was needed in total for each simulated shorter than the experimental results presented a rathercase. During the whole simulation process, the selection of difficult obstacle to overcome in the simulations. How-the appropriate force field was a crucial task for obtaining ever, taking N=60 to represent the whole polymer chainaccurate information about the structures and dynamics of for PMMA appeared a reasonable approach. Hence, thethe blends. The COMPASS force field has been shown to be minimum representative polymer chain lengths of PS anda suitable choice for calculating solubility parameters, PMMA, Nmon(PS) and Nmon(PMMA), were chosen to beespecially for polymeric systems . 30 and 60, respectively. Figure 3 shows a flowchart that illustrates the process described above.Results and discussion The blend systems were binary, with PS (density = 1.05 gcm−3) and PMMA (density = 1.188 g cm−3) as theThe cohesive energy density (CED) of each pure compo- components. The glass transition temperature of PS isnent was used to calculate the solubility parameter, δ,according to the equation below: rﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Ecohd ¼ CED ¼ ; V To determine the minimum representative polymer chainlength of the blend components, Nmon, cases with differentchain lengths, N=10, 20, 30, 40, 50, 60, 70 and 80 for bothPS and PMMA, were selected in order to calculate the δvalue of each component. Figure 1 displays the dependenceof δ of PS on the number of repeating units of PS. It can beseen that a nearly constant value is approached when thenumber of repeating units reaches 30, and the values are8.32% smaller than the experimental data. This may resultfrom the presence of a bulky C6H5 group in PS, whichrestricts free rotation around the C–C bond of its backbone.Figure 2 shows the calculated δ values for different Fig. 2 The solubility parameter for different PMMA chain lengths
610 J Mol Model (2011) 17:607–619 chains were randomly distributed in the simulation box, the model was assumed to be a well-mixed model and accepted for further simulations; otherwise, it was discarded, and a new blending model was built until the component chains contacted each other sufficiently. Figure 4 shows a typical 1/1 blend. Because of the end–end interactions of short polymer chains, the initial amorphous structure of the blend must first be minimized. The subsequent simulation process was the same as that used to calculate δ values for the pure components, and the simulation temperatures were also 383, 413 and 443 K. The tendency for binary polymer chains to mix depends on the cohesive energies of the blends and their pure components. Both are applied to calculate the χ parameters of blends with different compositions. The χ parameter is defined as ΔEmix χ¼ Vmon ; RT where Vmon is the unit volume of one monomer. Here, Vmon equals 165.54 cm3 mol−1 for blends of PS/PMMA. ΔEmix for a binary mixture is defined as Ecoh Ecoh Ecoh ΔEmix ¼ f1 þ f2 À ; V pure1 V pure2 V mix where f is the volume fraction, and the subscripts “pure” and “mix” denote the cohesive energy densities of the pure components and the binary mixture, respectively. χ is shown as a function of the PS volume fraction in Fig. 5. Several features of these data are impressive. Firstly, the three χ curves vary in almost the same way at different temperatures, which means that temperature was not an efficient factor for changing the degree of phase separation. This is a totally different conclusion from that obtained for PEO/PMMA blends, which are miscible . Secondly, the χ value shows a decreasing trend as the volume fraction of PS increases, except for the 1/4 blend case, where it shows a small risingFig. 3 The procedure used to select Nmon for PS trend. Then the 4/1, 6/1 and 8/1 blend cases also show another decreasing trend in χ. These two decreasing trends are termed T1 and T2, respectively. Considering the absolute data on373 K, so PS is prone to crystallize at a low temperature. slope variation for T1 and T2, where T1 T2, it is supposedPMMA starts to soften at the glass transition temperature that the degree of phase separation would intensify with(Tg =378 K), and does not substantially depolymerize until increasing PS content when the blends have a higher content453 K . Therefore, the blending simulation temper- of PS. In addition, the 1/4 and 4/1 blend cases producedatures adopted were 383, 413 and 443 K. outstandingly high χ values for both the T1 and the T2 lines, PS/PMMA blends with different weight percentages of which means that it is possible that extremely distinct phasePS were put in a three-dimensional (3D) periodic boundary separation was present in these two blend cases.simulation box with the corresponding density. Table 1 A positive χ value alone cannot prove that the blends aredescribes the blending models in detail, including the molar immiscible; it is necessary to calculate the critical value ofratios of PS to PMMA, the chain number per unit cell, the χ via the equation below:compositions by weight, and the densities. The blendproperties calculated in subsequent studies depend on how 2well the components are blended. Therefore, when the 1 1 1 ð χ AB Þcritical ¼ pﬃﬃﬃﬃﬃﬃﬃ þ pﬃﬃﬃﬃﬃﬃ ;blending model was generated, if the PS and the PMMA 2 mA mB
J Mol Model (2011) 17:607–619 611Table 1 Details of thePS/PMMA blend cases carried Number System Content wt% of PMMA p(gcm−3)out via MD simulation 1 Pure PMMA 1PMMA chain 100 1.1880 2 1/6 1PS, 6PMMA 92.02 1.1772 3 1/4 1PS, 4PMMA 88.49 1.1724 4 1/3 1PS, 3PMMA 85.22 1.1681 5 1/2 1PS, 2PMMA 79.36 1.1604 6 1/1 1PS, 1PMMA 65.78 1.1429 7 2/1 2PS, 1PMMA 49.01 1.1220 8 3/1 3PS, 1PMMA 39.06 1.1099 9 4/1 4PS, 1PMMA 32.46 1.1021 10 6/1 6PS, 1PMMA 24.27 1.0925 11 8/1 8PS, 1PMMA 19.38 1.0868 12 Pure PS 1PS chain 0 1.0500where mA and mB represent the actual number of repeating mixing ΔHm, could be used to characterize the miscibilityunits of PS and PMMA, respectively. When the calculated of polymer blends .and the critical values of χ are based on the same reference However, it is also necessary to calculate thermodynamicvolume, χAB)critical can be used to estimate the compatibil- parameters such as entropy, enthalpy and Gibbs free energyity of the blends. The blends are miscible if (χAB)calculated (G) to illustrate the phenomenon of polymer blending. The(χAB)critical. In this case, the Gibbs free energy, ΔGm, is entropy change upon mixing long polymers is so small thatnegative. In contrast, when (χAB)calculated ≫ (χAB)critical, the the mixing enthalpy becomes a key influence on the degreeblends are totally immiscible; the phases will even separate. of mixing. The entropy change upon mixing, ΔSm, must beWhen the difference between χAB)calculated and χAB)critical is considered in addition to the enthalpy of mixing. Hence, itsmall or even zero, the blends will be partially or even was important to compute ΔHm in order to study thetotally miscible. The value of χAB)critical in our studied PS/ miscibilities of the PS/PMMA blends using the followingPMMA blends was 0.0486, which was much smaller than equation :the calculated χ values. Therefore, we can see that the PS/PMMA blends were immiscible at 383, 413 and 443 K. hn oi2 ΔHm ¼ Vm ðCEDÞ0:5 ÀðCEDÞ0:5 fPSfPMMA; As long as the calculated χAB and the corresponding PS PMMAcritical values are based on the same reference volume,comparing the calculated χAB with critical values will where Vm is the total volume of the blend. The CED valuesprovide useful information about the degree of miscibility used to compute ΔHm were obtained from the data in theof the blends. Therefore, χAB, rather than the enthalpy of MD simulations.Fig. 4 Amorphous cell from the1/1 PS/PMMA blend case.Red, O; gray, C; white, H
612 J Mol Model (2011) 17:607–619 they exhibit the strongest attractive or repulsive interactions. Because of the low entropy of mixing, polymeric blends are mostly incompatible, and their phases will separate under the appropriate conditions. Therefore, it is necessary to carry out further research from a dynamic point of view at the mesoscopic level to study how the phase separations of PS/PMMA blends are influenced by certain inducing effects. Mesoscopic simulation PS/PMMA blends with a block copolymer and a shear field To map the representative polymer chains onto Gaussian chains, the bead number (Nmeso) and the unit chain lengthFig. 5 Flory–Huggins interaction parameter χ as a function of the PSvolume fraction for binary blends of PS/PMMA at 383, 413 and of the Gaussian chain (ameso) are estimated by443 K, respectively N mon Nmeso ¼ ; C1 To calculate ΔGm, the change in entropy during mixing, ameso ¼ amon C1;ΔScomb was needed, and this was calculated using the mcombinatorial entropy term for binary systems via Flory– where Nmon is the number of repeating units in the polymerHuggins theory  for two-component systems, as given by chain. amon is the reference unit monomer length, and C∞ is the characteristic ratio of a chain of infinite length. NmonΔScomb ¼ ÀR½# A ln # A þ # B ln # B : m was determined by the representative chain lengths of PS and PMMA, i.e., Nmon =30 for PS (MW =3200) and Nmon = Thus, by using the thermodynamic formula 60 for PMMA (MW =6000), while C∞(PS)=9.85 and C∞ (PMMA)=8.65 were found in the Polymer Handbook .ΔGm ¼ ΔHm À T ΔScomb ; m The connection between the microscale and the mesoscaleit was possible to calculate the Gibbs free energy of mixing. is as follows:Both ΔGm and ΔHm exhibited similar trends at 413 K overthe entire composition range, as shown in Fig. 6. The vÀ1 ij ¼ # AB RT ;extreme values of these two curves both appeared in the 1/1blend case. It is presumed that when the molar proportions where the parameter χAB is calculated by atomisticof PS and PMMA are the same, such as in the 1/1 blend, simulation for each blend composition at different temper- atures. R is the molar gas constant, 8.314 J mol−1 K−1, and T is the simulation temperature. The calculated χ values for various compositions were all positive at 383, 413 and 443 K. Nmeso and ν−1εij are the input parameters used in MesoDyn simulations to describe the number of Gaussian beads and the interaction between beads. In the 1/1 blend case, the Nmeso values for PS and PMMA were 3 and 6, respectively. In order to stabilize the numerical calculation, the time step for MesoDyn calculation, τ, was chosen to be 100 ns, and the total simulation time was 1000 μs for each blend case. A default noise parameter value of 75.002 was used for numerical speed and stability. The grid dimensions adopted were 32×32×32 nm. Ten mesoscopic simulations were carried out with different PS/PMMA blend composi- tions, 1/1, 1/2, 1/3, 1/4, 1/6, 2/1, 3/1, 4/1, 6/1 and 8/1 inFig. 6 Changes in enthalpy ΔHmix (solid curve) and Gibbs free molar ratio, which roughly covered the whole compositionenergy ΔGmix (dotted curve) with volume fraction of PS range.
J Mol Model (2011) 17:607–619 613Results and discussionThe order parameter, denoted P, is defined as the averagedifference between the local density squared and the overalldensity squared, as given by the equation Z 1 Â ÃPi ¼ h2 ðrÞ À h2 dr; i i V Vwhere ηi is the dimensionless density (volume fraction) ofspecies i. The larger the value of the order parameter, thestronger the phase separation. A decrease in P indicatesbetter compatibility or miscibility, and the polymer phasesmix more randomly. It should be pointed out that the P data calculated bymesoscopic simulation can only be compared for the same Fig. 7 V ROP value versus volume fraction of PS for ten blend casesblend composition. Therefore, plain PS/PMMA blends with 26 block copolymers added. The zero point on the Y axis was setwere used as reference cases, and their order parameter as the reference line. When the data are above this line, it means that the block copolymer has an enhancing effect on the PS/PMMA blend;data were labeled “A;” in addition, the order parameter data when the data are below this line, it has a deteriorating effect on theof PS/PMMA blends of the same compositions as for the blend. Isodensity surface pictures of a 6/1 (PS/PMMA) blend at 443,“A” blends but with inducing effects, such as being doped 413 and 383 K are displayed from top to bottom in the chart,with a block copolymer or nanoparticles, or having planes respectively. Red, PS; green, PMMAintroduced, were labeled “B.” The value of (B − A)/A istermed the variation rate of order parameters (V ROP for value of the 3/1 blend case also turned from positive toshort). By comparing the V ROP values, we can detect negative. Based on this information, and using the 1/1which factor is the most effective at changing the phase blend case as a reference, the V ROP values of pairs ofmorphology. blend cases (such as the 1/3 and 3/1 blend cases) turned In order to study the influence of the addition of a block from positive to negative as the temperature was graduallycopolymer on the phase morphology, a block copolymer increased. Following this principle, when the temperaturemade of PS and PMMA with a volume fraction of 10% was was raised above 443 K, the V ROP values of the 1/4 and 4/added to each blend. Generally speaking, when block 1 blend cases would be expected to become negative. Thecopolymers of the same composition are added to an three pictures inserted into Fig. 7 are the phase morphol-immiscible blend, the compatibility of the blend will be ogies of the 6/1 blend case with block copolymers added atenhanced. However, in our study, two opposite results were 443, 413 and 383 K (top to bottom, respectively).obtained when the block copolymer was added: an In order to investigate the influence of the shear field onenhancement of or a deterioration in compatibility were the microscopic phase morphology, the shear rate was set toboth observed. 0.001 ns−1 and 0.002 ns−1 as examples of low and high Several striking features of these data can be seen in shear effects. Simulations were then performed on the basisFig. 7. First, the V ROP values of blends with less PS (the of plain PS/PMMA blends with P data used as a reference.1/1, 1/2, 1/3, 1/4, 1/6, 2/1 and 3/1 blend cases) fluctuated It can be seen from Fig. 8 that low shear stress can have aaround zero, and this trend was most obvious for the 1/1, 1/ significant inducing effect on PS-rich blends, such as in the3 and 1/6 blend cases, which means that adding a block 4/1 and 6/1 blend cases. Phase separation can clearly becopolymer to the blends with less PS did not result in an seen in the inserted pictures. However, shear stress had noobvious inducing effect. However, obvious enhancing obvious effect on the 8/1 blend case. When the shear rateeffects were seen for the blends with more PS (the 4/1, 6/ was increased to 0.002 ns−1, all of the V ROP values for the1 and 8/1 blend cases). This result can be attributed to the ten different blend cases were high, as shown in Fig. 9,difference in the self-diffusion coefficients between PS and which means that high shear stress plays an important rolePMMA and the difference in their self-compatibility in changing the microscopic phase morphology, especiallyproperties. Second, the V ROP values of the 1/2, 1/1 and in PS-rich blends. In addition, the V ROP value of the 8/12/1 blend cases were negative at 383 K; when the blend case was relatively high. Furthermore, the phasetemperature was increased to 413 K, the V ROP value of morphologies of all the blends exhibited obvious phasethe 1/3 blend case turned from positive to negative. When separation. In a word, the higher the shear rate, the morethe temperature was raised again, to 443 K, the V ROP obvious the phase separation.
614 J Mol Model (2011) 17:607–619 Column-shaped nanoparticles were applied as an exam- ple. In order to determine the factor that exerts the most influence on phase separation, seven different kinds of nanoparticles were made for the doping study. In Table 2, the number of nanoparticles in each layer (Np), the radius of each nanoparticle (rp), the height of each nanoparticle (hp), the number of layers (NL) and the total number of nanoparticles doped (Ntp) are listed in detail. Among these cases, the 4-3-4-2 case (with four nanoparticles in each of two layers, a nanoparticle radius of 3 nm, and a nano- particle height of 4 nm) was used as a reference, and all the other cases were derived from this. For example, adding only one more nanoparticle in the center resulted in the 4-3- 4-3 case; increasing the number of layers to four but not changing any other settings yielded the 4-3-4-4 case;Fig. 8 V ROP data based on plain blends versus the volume fractionof PS. Isodensity surface pictures of a 4/1 (PS/PMMA) blend induced doubling the nanoparticle density of each layer producedby a shear rate of 0.001 ns−1 are also shown, as are isodensity surface the 8-3-4-2 case; doubling the nanoparticle height yieldedpictures of a 4/1 (PS/PMMA) blend at 383, 443 and 413 K (top to the 4-3-8-2 case; adding one more nanoparticle to the middlebottom in the chart, respectively). Red, PS; green, PMMA of the simulation box and increasing the number of layers to three on the basis of the 4-3-8-2 case produced the 4-3-8-3PS/PMMA blends doped with nanoparticles case; and doubling the nanoparticle radius on the basis of the 4-3-8-2 case gave the 4-6-8-2 case. The parameters chosenThe pairs of blend cases, such as the 1/3, 3/1 and the 1/2, 2/ were the same as those used in the previous mesoscopic1 blend pairs, were then used as examples to study the simulations; the χ value was that obtained at 400 K, andinducing effect of doping with nanoparticles. In addition, the total simulation time was 10 ms in each case. The simu-the 1/3 (with a PS volume fraction of 16.21%) and 1/2 lation models were the plain PS/PMMA blends shown in(with a PS volume fraction of 22.49%) blend cases were Table 1.used to represent compositions rich in PMMA, while the 2/1 (with a PS volume fraction of 53.72%) blend case was Result and discussionused to represent compositions that contain roughly equalamounts of PS and PMMA, and the 3/1 (PS volume Figure 10 shows the V ROP values obtained for variousfraction of 63.52%) blend case was chosen to represent kinds of nanoparticle doping situations. A few trends can becompositions rich in PS. seen in these cases. First, the trends seen in these four pictures are almost the same. Second, since V ROP1/3 V ROP1/2 V ROP2/1 V ROP3/1, it can be deduced that the degree of phase separation intensifies with increasing PMMA content when the blend is rich in PMMA. Third, since V ROP4-3-4-3 V ROP4-3-4-2 and V ROP4-3-8-3 V ROP4-3-8-2, the order of the PS/PMMA blend increases when the number of nanoparticles of the same size is Table 2 Mesoscopic simulations of PS/PMMA blends doped with nanoparticles Simulation Case Np rp (nm) hp (nm) NL Ntp 1 4-3-4-2 4 3 4 2 8 2 4-3-4-3 4 3 4 3 9 3 4-3-4-4 4 3 4 4 16 4 4-3-8-2 4 3 8 2 8Fig. 9 V ROP data with the shear effect versus the volume fraction ofPS. Isodensity surface pictures of an 8/1 (PS/PMMA) blend induced 5 4-3-8-3 4 3 8 3 9by a shear rate of 0.002 ns−1 are also shown, as are isodensity surface 6 4-6-8-2 4 6 8 2 8pictures of an 8/1 (PS/PMMA) blend at 443, 413 and 383 K (top to 7 8-3-4-2 8 3 4 2 16bottom in the chart, respectively). Red, PS; green, PMMA
J Mol Model (2011) 17:607–619 615Fig. 10 V ROP data for the 1/2, 2/1 and the 1/3, 3/1 blend pairs doped with nanoparticles at 383, 413 and 443 Kincreased. Fourth, since V ROP8-3-4-2 V ROP4-3-4-4, the From the third, fourth and fifth results discussed aboveorder of the PS/PMMA blend can be increased by (V ROP4-6-8-2 ≫ V ROP8-3-4-2 V ROP4-3-4-4 V ROP4-3-8-3increasing the density of the nanoparticles of the same V ROP4-3-8-2 VROP4-3-4-3 V ROP4-3-4-2), we can seesize. Fifth, it can be seen from the extremely high value of that the factors investigated had the following order ofV ROP4-6-8-2 that the nanoparticle size is the factor that influence on the phase separation: nanoparticle size exerts the most influence on the phase morphology. nanoparticle density number of doped nanoparticles.Table 3 Mesoscopic simulationsof PS/PMMA blends induced “ci” type Row number (X-axis) Row number (Y-axis) Radius (nm)by “ci” and “co” planes ci-444 4 4 4 ci-882 8 8 2 “co” type E/Tg (X-axis) E/Tg (Y-axis) Height (nm) co-444 2/4 2/4 4 co-448 2/4 2/4 8 co-4412 2/4 2/4 12 co-4432 2/4 2/4 32 co-884 4/8 4/8 4 co-888 4/8 4/8 8 co-8812 4/8 4/8 12g This is the abbreviation for co-8832 4/8 4/8 32“effective/total row number.”
616 J Mol Model (2011) 17:607–619Table 4 Mesoscopic simulationsof PS/PMMA blends induced “gra” type Row number (X-axis) Height (nm) Sfin X-axisby “gra” and “rg” planes gra-444 4 4,3,2,1 N gra-888 8 8,7,6,5,4,3,2,1 N gra-2(444) 8 4,3,2,1,1,2,3,4 Y gra-2(448) 8 8,4,2,1,1,2,4,8 Y gra-2(888) 16 8,7,6,5,4,3,2,1,1,2,3,4,5,6,7,8 Y “rg” type Layer number Height (nm) Sf in the X- and Y-axes rg-442 2 2,4 Yf This is the abbreviation for rg-884 4 8,4,2,1 Y“symmetry;” “N” means “no” and rg-16168 8 16,14,12,10,8,6,4,2 Y“Y” means “yes”Furthermore, all of the PS/PMMA blend cases showed the vigorous phase separation on rougher planes. Thesame trends as those described above with nanoparticle values of V ROPco-884 and V ROPco-888 were almostdoping. the same at 383, 413 and 443 K. The values of V ROPco-8812 at 383 and 413 K were also the same, butPS/PMMA blends induced by various planes the value of V ROPco-8812 at 443 K jumped to 13.3, which was one order of magnitude higher than itsTo investigate which planes induce the most intense phase values at 383 and 413 K. On a much rougher surface,separation in PS/PMMA blends, four different types of such as a co-8832 type of plane, V ROPco-8832,443K inducing planes were designed as substrates using our own V ROPco-8832,413K V ROPco-8832,383K, which revealsprogram. These four types were denoted “ci,” “co,” “gra,” that PS/PMMA blends undergo more intense phaseand “rg.” The “ci” series of planes used half-spheres with separation at higher temperatures. The surfaces of thedifferent radii as a mask that simulated different degrees of co-4xx series of planes were rougher than those of the co-surface roughness. The “co” series had equally spaced 8xx series of planes. The V ROP values of the co-4xxcubic columns as a mask. The columns had different sizes series were higher than those of the co-8xx series atand heights to simulate different degrees of surface 443 K, which is also consistent with the conclusion thatroughness. The “gra” series were planes with different more intense phase separation occurs on rougher planes.widths to simulate different degrees of surface roughness. (2) For the “ci” planes, V ROPci-882 V ROPci-444 at theThe mask was generated by gradually increasing the same temperature. There was no obvious differencecolumn height across the plane, so that it resembled stairs between the V ROPci-882 values at 383 and 443 K, andviewed side on. In addition, monodirectional asymmetric there was no obvious difference between the V ROPci-planes, such as gra-444 and gra-888, and monodirectional 444 values at 383 and 443 K either. Furthermore, the Vsymmetric planes, such as gra-2(444), gra-2(448) and gra-2 ROPci-882 and V ROPci-444 values at 413 K were both(888), were considered. The “rg” series were bidirectional higher than their corresponding values at lowersymmetric planes originating from monodirectional sym- (383 K) or higher (443 K) temperatures. This showsmetric planes, as used in the “gra” series. Tables 3 and 4 that temperature is the most influential factor on thedescribe these four types of planes used in the simulations, phase separation of PS/PMMA blends induced by “ci”and Fig. 11 shows the eighteen planes pictorially. planes, but also that the V ROP values vary irregularly with temperature. Both the temperature and the degreeResults and discussion of surface roughness contribute to the results. (3) For the “rg” planes, the same order of V ROPrg-16168 Figure 12 shows the V ROP values of PS/PMMA blends V ROPrg-884 V ROPrg-442 was seen at three temper-induced by the four types of planes mentioned above; atures, which shows that the degree of surface roughnesseighteen isodensity surface pictures are shown for the 1/3 is an important factor for inducing phase separation,blend case at 413 K as examples at the top of each chart. especially for rougher planes with high step gradients,The following trends can be discerned from these figures: such as rg-16168. Nearly the same value of V ROPrg-442 was observed at 383 and 443 K—the same situation as(1) For the “co” planes, V ROPco-8832 V ROPco-8812 V seen for V ROPrg-884—so it can be presumed that for ROPco-888 V ROPco-884 and V ROPco-4432 V the smoother planes, such as rg-884 and rg-442, ROPco-4412 V ROPco-448 V ROPco-444, which temperature is more important than the degree of shows that the PS/PMMA blends underwent more surface roughness in inducing phase separation.
J Mol Model (2011) 17:607–619 617Fig. 11 The four types of plane used in the simulations: “ci,” “rg,” “gra,” and “co”(4) For the “gr” planes, the V ROP values for gr-444 were surface roughness plays a small role in inducing phase lower than those for other “gr” planes at 383, 413 and separation for “gr” planes. In contrast, it can be deduced 443 K, and all of these planes presented similar values at from the extremely high value of V ROP at 413 K that 383 and 443 K; in addition, the other “gr” planes except temperature is the main inducing factor for these planes. for gr-444 presented nearly the same V ROP values at (5) For all of the “ci,” “rg,” and “gr” planes, the V ROP 383, 413 and 443 K. This shows that the degree of values at 413 K were much higher than those at 383
618 J Mol Model (2011) 17:607–619Fig. 12 V ROP data for the 1/3 blend case at 383, 413 and 443 K, respectively. Isodensity surface pictures are shown for PS/PMMA blendsinduced by different types of planes at 413 K. Red, PS; green, PMMA and 443 K; furthermore, the V ROP values at 383 and and spread; they could only adjust themselves in the “small 443 K were nearly the same for each plane, which cubic spaces” formed by neighboring column masks. reveals that using a higher (443 K) or lower (383 K) Furthermore, the big difference between the diffusion temperature had nearly the same effect on phase abilities of PS and PMMA was also a barrier to movement separation, and that there was a “critical” temperature and adjustment. Because of the two reasons mentioned between 443 and 383 K (such as 413 K) that could above, the degrees of phase separation differed widely induce the most vigorous phase separation. The between the first three types of plane and the “co” planes. influence of each “ci,” “rg,” or “gr” plane on phase separation mainly depended on this critical tempera- ture, not on the degree of surface roughness, in Conclusion contrast to what was seen for the “co” planes. The two most important processes during the MD simula- The “ci,” “rg,” and “gr” planes were different from the tion are the annealing process after minimization and the“co” planes in that the first three types of plane had MD simulations with three NVT and NPT ensemble cycles.continuous mask distributions on their surfaces, which The strong polymer end–end interactions, which evidentlyallowed the PS/PMMA blends to move and spread more influence the simulation results, can only be reduced byfreely until they could adjust themselves to reach stable performing the above two processes. Based on thephase separation. In contrast, the “co” planes did not have calculated δ values for different numbers of repeating unitscontinuous mask distributions on their surfaces, which of PS and PMMA, their representative chain lengths weremeant that the polymer did not have enough room to move found to be 30 and 60, respectively. By comparing the
J Mol Model (2011) 17:607–619 619calculated χ with χcritical, it was found that the PS/PMMA 2. Abd-El-Messieh SL (2003) Polym Plast Technol Eng 42(1):153–169blends were immiscible in our simulations. Furthermore, 3. Schneider IA, Calugaru EM (1976) Eur Polym J 12(12):879–881 4. Bada R, Perez Jubindo MA, De LA, Fuente MR (1987) Materthe χ data did not depend greatly on the simulation Chem Phys 18(4):359–373temperatures. 5. Zhu PP (1997) Eur Polym J 33(3):411–413 The input parameters used in MesoDyn were derived from 6. Lee JK, Han CD (1999) Polymer 40:6277–6296the MD simulations, and mesoscopic simulations were carried 7. Lee CF (2000) Polymer 41(4):1337–1344 8. Li X, Han YC, An LJ (2003) Polymer 44(26):8155–8165out at 383, 413 and 443 K. After calculating the V ROP values 9. Walheim S, Boltau M, Mlynek J, Krausch G, Steiner U (1997)of ten different representative composition cases with block Macromolecules 30:4995–5003copolymer added, two outstanding features were found. 10. Schmidt JJ, Gardella JA Jr, Salvati L Jr (1989) MacromoleculesFirst, the PS-rich blend cases at higher simulation temper- 22:4489–4495 11. Chiou JS, Barlow JW, Paul DR (1987) J Polym Sci Part B Polymatures, such as 413 and 443 K, underwent a more obvious Phys 25:1459–1471phase separation in microscopic phase morphology. Second, 12. Lhoest JB, Bertrand P, Weng LT, Dewez JL (1995) Macro-when the 1/1 blend case was used as the reference, the molecules 28:4631–4637symmetric blend pairs, such as 1/2, 2/1 and 1/3, 3/1, etc., 13. Davies MC, Shakesheff KM, Shard A, Domb A, Roberts CJ, Tendler SJB, Williams PM (2000) Macromolecules 29:2205–2212gradually showed miscibility as the temperature was increased. 14. Schreiber HP (1993) Aspects of component interactions in Mesoscopic simulations were then carried out on PS/ polymer systems: the interfacial interactions in polymeric compo-PMMA blends with shear stress factored in. The results of sites. Kluwer, Bostonthose simulations showed that this shearing was a good way of 15. Buki L, Gonczy E, Fekete E, Hellmann GP, Pukanszky B (2001) Macromol Symp 170:9–20inducing phase separation, especially in PS-rich blends. Here, 16. Lodge TP, Wood ER, Haley JC (2006) J Polym Sci Part B Polymthe temperature was not found to be an important factor in Phys 44:756–763phase separation, especially for the PMMA-rich blends. 17. Valls OT, Farrell JE (1993) Phys Rev E 47:R36–R39 Next, mesoscopic simulations were carried out on plain 18. Ramirez-Piscina L, Hernandéz-Machado A, Sancho JM (1993) Phys Rev B 48:125–131PS/PMMA blends doped with various numbers and densities 19. Kawakatsu T, Kawasaki K, Furusaka M, Okabayashi H, Kanaya Tof nanoparticles of various sizes. The simulation results (1993) J Chem Phys 99(10):8200–8217showed that nanoparticle doping was an effective way of 20. Shinozaki A, Oono Y (1993) Phys Rev E 48:2622–2654improving the degree of order in the microscopic phases, 21. Fraaije JEM (1993) J Chem Phys 99:9202–9212 22. Fraaije JGEM, van Vlimmeren BAC, Maurits NM, Postma M,especially in the PMMA-rich blends. No matter which PS/ Evers OA, Hoff-man C, Altevogt P, Goldbeck-Wood G (1997)PMMA blend composition was considered, the nanoparticle J Chem Phys 106:4260–4269size had a stronger influence on the phase morphology than 23. Jawalkar SS, Adoor SG, Sairam M, Nadagouda MN, Aminabhavi TMthe density of nanoparticles, and the density of nanoparticles (2005) J Phys Chem B 109(32):15611–15620 24. Groot RD, Warren PB (1997) J Chem Phys 107:4423–4435had a stronger influence than the number of nanoparticles. 25. Groot RD, Madden TJ (1998) J Chem Phys 108:8713–8724 Finally, in order to research the effects of various planes on 26. Mu D, Huang XR, Lu ZY, Sun CC (2008) Chem Phys 348:122–129the phase separation of PS/PMMA blends, four types (“ci,” 27. Flory PJ (1989) Statistical mechanics of chain molecules. Munich,“rg,” “gr” and “co”) of planes were constructed. For the first Germany 28. Mark JE (1999) Polymer data handbook. Oxford University Press,three types of planes, the degree of surface roughness played New Yorkonly a small role in inducing phase separation: the temperature 29. Brandrup J, Immergut EH, Grulke EA (1999) Polymer handbook,was the most important factor in this respect. Furthermore, 4th edn. Wiley, New Yorkthere was a “critical” temperature between 443 and 383 K 30. Hoover WG (1985) Phys Rev A 31:1695–1697 31. Rigby D, Sun H, Eichinger BE (1997) Polym Int 44:311–330(such as 413 K) at which the phase separation occurred most 32. Sun H (1998) J Phys Chem B 102:7338–7364intensely. However, rougher planes and higher temperatures 33. Sun H, Ren P, Fried JR (1998) Comput Theor Polym Sci 8:229–246both helped to induce phase separation on “co” planes. 34. Ewald PP (1921) Ann Phys 64:253–287 35. Grulke EA (1999) Solubility parameter values. In: Polymer handbook, 4th edn. Wiley, New York 36. Calahorra E, Cortazar M, Guzman GM (1985) J Polym Sci Polym Lett Ed 23:257–260References 37. Krause S, Paul DR, Newman S (1978) Polymer–polymer compatibility in polymer blends, vol 1. Academic, New York 1. Paul DR, Newman S (1978) Polymer blends. Academic, New 38. Fan CF, Cagin T, Chen ZM, Smith KA (1994) Macromolecules York 27:2383–2391